LMucko/crystallography-open-database huggingface dataset:
Halite-sylvite thermoelasticity Sample: r54935, T = 450 C, P = 8.8 kbar, cell volume = 223.47 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003185
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r54935, T = 450 C, P = 8.8 kbar, cell volume = 223.47 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.6Na.4)Cl
_chemical_formula_sum            'Cl K0.6 Na0.4'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.0684
_cell_length_b                   6.0684
_cell_length_c                   6.0684
_cell_volume                     223.472
_cell_formula_units_Z            4
_database_code_amcsd             0003274
_diffrn_ambient_pressure         8.8e+05
_diffrn_ambient_temperature      723.15
_exptl_crystal_density_diffrn    2.024
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.6 Na.4) Cl'
_cod_database_code               9003185
_amcsd_formula_title             (K.6Na.4)Cl
Halite-sylvite thermoelasticity Sample: r54883, T = 450 C, P = 8.9 kbar, cell volume = 223.54 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003186
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r54883, T = 450 C, P = 8.9 kbar, cell volume = 223.54 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.6Na.4)Cl
_chemical_formula_sum            'Cl K0.6 Na0.4'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.0690
_cell_length_b                   6.0690
_cell_length_c                   6.0690
_cell_volume                     223.538
_cell_formula_units_Z            4
_database_code_amcsd             0003275
_diffrn_ambient_pressure         8.9e+05
_diffrn_ambient_temperature      723.15
_exptl_crystal_density_diffrn    2.024
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.6 Na.4) Cl'
_cod_database_code               9003186
Halite-sylvite thermoelasticity Sample: r54807, T = 450 C, P = 15.7 kbar, cell volume = 216.44 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003187
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r54807, T = 450 C, P = 15.7 kbar, cell volume = 216.44 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.6Na.4)Cl
_chemical_formula_sum            'Cl K0.6 Na0.4'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.0041
_cell_length_b                   6.0041
_cell_length_c                   6.0041
_cell_volume                     216.443
_cell_formula_units_Z            4
_database_code_amcsd             0003276
_diffrn_ambient_pressure         1.57e+06
_diffrn_ambient_temperature      723.15
_exptl_crystal_density_diffrn    2.090
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.6 Na.4) Cl'
_cod_database_code               9003187
Halite-sylvite thermoelasticity Sample: als13k60, T = 500 C, P = 0.0 kbar, cell volume = 237.83 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003188
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als13k60, T = 500 C, P = 0.0 kbar, cell volume = 237.83 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.6Na.4)Cl
_chemical_formula_sum            'Cl K0.6 Na0.4'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.1957
_cell_length_b                   6.1957
_cell_length_c                   6.1957
_cell_volume                     237.832
_cell_formula_units_Z            4
_database_code_amcsd             0003277
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    1.902
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.6 Na.4) Cl'
_cod_database_code               9003188
_amcsd_formula_title             (K.6Na.4)Cl
Halite-sylvite thermoelasticity Sample: r54907, T = 500 C, P = 9.8 kbar, cell volume = 223.50 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003189
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r54907, T = 500 C, P = 9.8 kbar, cell volume = 223.50 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.6Na.4)Cl
_chemical_formula_sum            'Cl K0.6 Na0.4'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.0687
_cell_length_b                   6.0687
_cell_length_c                   6.0687
_cell_volume                     223.505
_cell_formula_units_Z            4
_database_code_amcsd             0003278
_diffrn_ambient_pressure         9.8e+05
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    2.024
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.6 Na.4) Cl'
_cod_database_code               9003189
_amcsd_formula_title             (K.6Na.4)Cl
Halite-sylvite thermoelasticity Sample: r54927, T = 500 C, P = 9.8 kbar, cell volume = 223.99 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003190
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r54927, T = 500 C, P = 9.8 kbar, cell volume = 223.99 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.6Na.4)Cl
_chemical_formula_sum            'Cl K0.6 Na0.4'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.0731
_cell_length_b                   6.0731
_cell_length_c                   6.0731
_cell_volume                     223.991
_cell_formula_units_Z            4
_database_code_amcsd             0003279
_diffrn_ambient_pressure         9.8e+05
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    2.020
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.6 Na.4) Cl'
_cod_database_code               9003190
_amcsd_formula_title             (K.6Na.4)Cl
Halite-sylvite thermoelasticity Sample: r54879, T = 500 C, P = 10.1 kbar, cell volume = 223.91 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003191
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r54879, T = 500 C, P = 10.1 kbar, cell volume = 223.91 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.6Na.4)Cl
_chemical_formula_sum            'Cl K0.6 Na0.4'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.0724
_cell_length_b                   6.0724
_cell_length_c                   6.0724
_cell_volume                     223.914
_cell_formula_units_Z            4
_database_code_amcsd             0003280
_diffrn_ambient_pressure         1.01e+06
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    2.020
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.6 Na.4) Cl'
_cod_database_code               9003191
_amcsd_formula_title             (K.6Na.4)Cl
Halite-sylvite thermoelasticity Sample: r52113, T = 500 C, P = 11.9 kbar, cell volume = 220.87 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003192
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r52113, T = 500 C, P = 11.9 kbar, cell volume = 220.87 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.6Na.4)Cl
_chemical_formula_sum            'Cl K0.6 Na0.4'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.0448
_cell_length_b                   6.0448
_cell_length_c                   6.0448
_cell_volume                     220.875
_cell_formula_units_Z            4
_database_code_amcsd             0003281
_diffrn_ambient_pressure         1.19e+06
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    2.048
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.6 Na.4) Cl'
_cod_database_code               9003192
_amcsd_formula_title             (K.6Na.4)Cl
Halite-sylvite thermoelasticity Sample: r54803, T = 500 C, P = 16.5 kbar, cell volume = 216.71 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003193
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r54803, T = 500 C, P = 16.5 kbar, cell volume = 216.71 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.6Na.4)Cl
_chemical_formula_sum            'Cl K0.6 Na0.4'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.0066
_cell_length_b                   6.0066
_cell_length_c                   6.0066
_cell_volume                     216.714
_cell_formula_units_Z            4
_database_code_amcsd             0003282
_diffrn_ambient_pressure         1.65e+06
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    2.087
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.6 Na.4) Cl'
_cod_database_code               9003193
_amcsd_formula_title             (K.6Na.4)Cl
Halite-sylvite thermoelasticity Sample: als12k60, T = 550 C, P = 0.0 kbar, cell volume = 240.18 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003194
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als12k60, T = 550 C, P = 0.0 kbar, cell volume = 240.18 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.6Na.4)Cl
_chemical_formula_sum            'Cl K0.6 Na0.4'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.2160
_cell_length_b                   6.2160
_cell_length_c                   6.2160
_cell_volume                     240.178
_cell_formula_units_Z            4
_database_code_amcsd             0003283
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      823.15
_exptl_crystal_density_diffrn    1.884
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.6 Na.4) Cl'
_cod_database_code               9003194
_amcsd_formula_title             (K.6Na.4)Cl
Halite-sylvite thermoelasticity Sample: r54875, T = 550 C, P = 11.2 kbar, cell volume = 224.59 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003195
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r54875, T = 550 C, P = 11.2 kbar, cell volume = 224.59 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.6Na.4)Cl
_chemical_formula_sum            'Cl K0.6 Na0.4'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.0785
_cell_length_b                   6.0785
_cell_length_c                   6.0785
_cell_volume                     224.589
_cell_formula_units_Z            4
_database_code_amcsd             0003284
_diffrn_ambient_pressure         1.12e+06
_diffrn_ambient_temperature      823.15
_exptl_crystal_density_diffrn    2.014
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.6 Na.4) Cl'
_cod_database_code               9003195
_amcsd_formula_title             (K.6Na.4)Cl
Halite-sylvite thermoelasticity Sample: r52105, T = 550 C, P = 12.6 kbar, cell volume = 221.26 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003196
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r52105, T = 550 C, P = 12.6 kbar, cell volume = 221.26 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.6Na.4)Cl
_chemical_formula_sum            'Cl K0.6 Na0.4'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.0483
_cell_length_b                   6.0483
_cell_length_c                   6.0483
_cell_volume                     221.259
_cell_formula_units_Z            4
_database_code_amcsd             0003285
_diffrn_ambient_pressure         1.26e+06
_diffrn_ambient_temperature      823.15
_exptl_crystal_density_diffrn    2.045
_cod_original_cell_volume        221.258
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.6 Na.4) Cl'
_cod_database_code               9003196
_amcsd_formula_title             (K.6Na.4)Cl
Halite-sylvite thermoelasticity Sample: r54795, T = 550 C, P = 17.3 kbar, cell volume = 216.88 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003197
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r54795, T = 550 C, P = 17.3 kbar, cell volume = 216.88 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.6Na.4)Cl
_chemical_formula_sum            'Cl K0.6 Na0.4'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.0081
_cell_length_b                   6.0081
_cell_length_c                   6.0081
_cell_volume                     216.876
_cell_formula_units_Z            4
_database_code_amcsd             0003286
_diffrn_ambient_pressure         1.73e+06
_diffrn_ambient_temperature      823.15
_exptl_crystal_density_diffrn    2.086
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.6 Na.4) Cl'
_cod_database_code               9003197
_amcsd_formula_title             (K.6Na.4)Cl
Halite-sylvite thermoelasticity Sample: als11k60, T = 600 C, P = 0.0 kbar, cell volume = 242.91 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003198
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als11k60, T = 600 C, P = 0.0 kbar, cell volume = 242.91 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.6Na.4)Cl
_chemical_formula_sum            'Cl K0.6 Na0.4'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.2395
_cell_length_b                   6.2395
_cell_length_c                   6.2395
_cell_volume                     242.912
_cell_formula_units_Z            4
_database_code_amcsd             0003287
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    1.862
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.6 Na.4) Cl'
_cod_database_code               9003198
_amcsd_formula_title             (K.6Na.4)Cl
Halite-sylvite thermoelasticity Sample: als5k60, T = 600 C, P = 0.0 kbar, cell volume = 242.26 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003199
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als5k60, T = 600 C, P = 0.0 kbar, cell volume = 242.26 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.6Na.4)Cl
_chemical_formula_sum            'Cl K0.6 Na0.4'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.2339
_cell_length_b                   6.2339
_cell_length_c                   6.2339
_cell_volume                     242.259
_cell_formula_units_Z            4
_database_code_amcsd             0003288
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    1.867
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.6 Na.4) Cl'
_cod_database_code               9003199
_amcsd_formula_title             (K.6Na.4)Cl
Halite-sylvite thermoelasticity Sample: als6k60, T = 600 C, P = 0.0 kbar, cell volume = 242.45 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003200
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: als6k60, T = 600 C, P = 0.0 kbar, cell volume = 242.45 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.6Na.4)Cl
_chemical_formula_sum            'Cl K0.6 Na0.4'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.2355
_cell_length_b                   6.2355
_cell_length_c                   6.2355
_cell_volume                     242.445
_cell_formula_units_Z            4
_database_code_amcsd             0003289
_diffrn_ambient_pressure         0
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    1.866
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.6 Na.4) Cl'
_cod_database_code               9003200
_amcsd_formula_title             (K.6Na.4)Cl
Halite-sylvite thermoelasticity Sample: r54911, T = 600 C, P = 11.5 kbar, cell volume = 224.17 ang**3
Walker, D.; Verma, P. K.; Cranswick, L. M. D.; Jones, R. L.; Clark, S. M.; Buhre, S.; American Mineralogist 89 (2004) 204–210; doi:

data_9003201
_publ_section_title
;
 Halite-sylvite thermoelasticity
 Sample: r54911, T = 600 C, P = 11.5 kbar, cell volume = 224.17 ang**3
;
_journal_name_full               'American Mineralogist'
_journal_page_first              204
_journal_page_last               210
_journal_volume                  89
_journal_year                    2004
_chemical_formula_structural     (K.6Na.4)Cl
_chemical_formula_sum            'Cl K0.6 Na0.4'
_space_group_IT_number           225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   6.0747
_cell_length_b                   6.0747
_cell_length_c                   6.0747
_cell_volume                     224.168
_cell_formula_units_Z            4
_database_code_amcsd             0003290
_diffrn_ambient_pressure         1.15e+06
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    2.018
_cod_original_sg_symbol_H-M      'F m 3 m'
_cod_original_formula_sum        '(K.6 Na.4) Cl'
_cod_database_code               9003201
_amcsd_formula_title             (K.6Na.4)Cl